liquid-infused structured surfaces with exceptional anti ... ?· liquid-infused structured...
Post on 19-Jul-2018
Embed Size (px)
Liquid-infused structured surfaces with exceptionalanti-biofouling performanceAlexander K. Epsteina, Tak-Sing Wonga,b, Rebecca A. Belisleb, Emily Marie Boggsa, and Joanna Aizenberga,b,c,1
aSchool of Engineering and Applied Sciences, Harvard University, 29 Oxford Street, Cambridge, MA 02138; bWyss Institute for Biologically InspiredEngineering, 3 Blackfan Circle, Boston, MA 02115; and cDepartment of Chemistry and Chemical Biology, Harvard University, 12 Oxford Street, Cambridge,MA 02138
Edited by Peter G. Wolynes, Rice University, Houston, TX, and approved July 3, 2012 (received for review February 3, 2012)
Bacteria primarily exist in robust, surface-associated communitiesknown as biofilms, ubiquitous in both natural and anthropogenicenvironments. Mature biofilms resist a wide range of antimicrobialtreatments and pose persistent pathogenic threats. Treatment ofadherent biofilm is difficult, costly, and, in medical systems suchas catheters or implants, frequently impossible. At the same time,strategies for biofilm prevention based on surface chemistry treat-ments or surface microstructure have been found to only transi-ently affect initial attachment. Here we report that Slippery Liquid-Infused Porous Surfaces (SLIPS) prevent 99.6% of Pseudomonasaeruginosa biofilm attachment over a 7-d period, aswell as Staphy-lococcus aureus (97.2%) and Escherichia coli (96%), under both sta-tic and physiologically realistic flow conditions. In contrast, bothpolytetrafluoroethylene and a range of nanostructured superhy-drophobic surfaces accumulate biofilm within hours. SLIPS showapproximately 35 times the reduction of attached biofilm versusbest case scenario, state-of-the-art PEGylated surface, and over afar longer timeframe. We screen for and exclude as a factor cyto-toxicity of the SLIPS liquid, a fluorinated oil immobilized on a struc-tured substrate. The inability of biofilm to firmly attach to thesurface and its effective removal under mild flow conditions (about1 cms) are a result of the unique, nonadhesive, slippery charac-ter of the smooth liquid interface, which does not degrade over theexperimental timeframe. We show that SLIPS-based antibiofilmsurfaces are stable in submerged, extreme pH, salinity, and UV en-vironments. They are low-cost, passive, simple tomanufacture, andcan be formed on arbitrary surfaces. We anticipate that our find-ings will enable a broad range of antibiofilm solutions in the clin-ical, industrial, and consumer spaces.
antifouling surfaces biofilm resistance slippery materials surface engineering
Bacteria in their natural state form biofilmsstructured, multi-cellular communities on surfaces in natural and anthropo-genic environments (1, 2). Biofilms contaminate a wide varietyof infrastructure elements, systems, and devices, such as plumb-ing, oil refineries, medical implants, food processing facilities,and heating and air conditioning networks (35). Marine fouling,which initiates the accumulation of bacterial biofilm on ship hullsfollowed by the attachment of larger marine organisms, increasesthe fuel burn of seafaring vessels by up to 40% (6). In medicalsettings, biofilms are the cause of persistent infectionsimpli-cated in 80% or more of all microbial casesreleasing harmfultoxins and even obstructing indwelling catheters. Such nosoco-mial infections affect about 10% of all hospital patients in theUnited States, result in nearly 100,000 deaths annually, and con-sequently drive much of current biotechnology research (79).
Biofilms protect their constituent cells in various ways, whichmakes both clinical and industrial contamination difficult and/orcostly to treat. As self-organized communities, biofilms haveevolved as differentiated cell phenotypes performing comple-mentary functions. The cooperative behavior of bacterial cells,mediated by cellcell communication and other factors, enablesan increased metabolic diversity and efficiency as well as an
enhanced resistance to environmental stresses, antimicrobialagents, and immune response. For example, some constituentcells are active in spreading the biofilm while others enter dor-mant states invulnerable to many antimicrobials (1013). Themacroscopic physical properties of biofilms, in which cells arebound together by a protein and exopolysaccharide matrix, alsoprotect them by resisting penetration of conventional liquid andvapor-phase antimicrobials (14). Indeed, the resistance to threatscovers a wide range of treatments. For example, exposure tochlorine bleach for 60 min still leaves live cells (8); biofilms inpipes flushed continuously with multiple biocides over 7 d reco-lonize the pipes (15), and biofilms can survive in bottled iodinesolution for up to 15 months (16).
Clearly, it is extremely desirable to prevent rather than treatbiofilm formation, and accordingly, a wide range of bacteria-resistant surfaces have been proposed. Most strategies rely eitheron a release of biocidal compounds or on inhibiting adhesion(1720). In the first case, techniques involve the design of coat-ings or bulk materials that release agents such as antibiotics, qua-ternary ammonium salts, and silver ions into the surroundingaqueous environment (19). The latter approach has focusedon the use of surface chemical functional groups that inhibit pro-tein adsorption as a means to inhibit bacterial adhesion. Exam-ples include low-surface-energy, weakly polarizable materials(e.g., Teflon) that minimize van der Waals interactions (21); zwit-terionic, mixed-charge, or amphiphilic materials (22) that utilizesurface inhomogeneities (e.g., charge and hydrophobicity) tofrustrate adhesion at the nano to micrometer scales (23); and hy-drophilic polymeric materials that form highly hydrated surfacesto inhibit protein adhesion (24). One of the most commonly stu-died hydrophilic modifications is poly(ethylene glycol), or PEG(25, 26). Solid/liquid/liquid antifouling interfaces based on com-plex coacervation and/or complex coacervate core micelles havealso been reported (2729). More recently, structured superhy-drophobic surfaces mimicking the Lotus leaf have been suggested(17, 30).
Each of these strategies, however, is generally transient.Materials that persistently resist bacteria are difficult to achieveby surface chemistry or surface structuring alone. The surfacemolecules are subject to desorption over time, a limitation thathas driven much research in the area of strengthening the phy-sisorption of, for example, PEG coatings (19). However, evenif no desorption occurs and bacteria are unable to attach directlyto a substrate, nonspecific adsorption of proteins and surfactantssecreted by bacteria can still mask the underlying chemical func-
Author contributions: J.A., A.K.E. and T.S.W. designed research; A.K.E., T.S.W., E.M.B. andR.A.B. performed research; A.K.E., T.S.W., R.A.B. and J.A. analyzed data; and A.K.E, T.S.W.and J.A. wrote the paper.
The authors declare no conflict of interest.
This article is a PNAS Direct Submission.
Freely available online through the PNAS open access option.1To whom correspondence should be addressed. E-mail: firstname.lastname@example.org.
This article contains supporting information online at www.pnas.org/lookup/suppl/doi:10.1073/pnas.1201973109/-/DCSupplemental.
1318213187 PNAS August 14, 2012 vol. 109 no. 33 www.pnas.org/cgi/doi/10.1073/pnas.1201973109
tionality (3133). Additionally, any defects in the surface chem-istry could serve as nucleation sites for bacterial attachment.Structured superhydrophobic surfaces in the Cassie (trappedair) state are prone to irreversible wetting (Wenzel transition),especially with the production of bacterial surfactant, seriouslylimiting their lifetime in submerged environments (34). Strategiesinvolving leaching of biocides are limited over a longer timescalebecause their reservoir is finite and subject to depletion (20).Also, the emergence of antibiotic- and silver-resistant pathogenicstrains, along with new restrictions on the use of biocide-releasingcoatings in the marine environment, has necessitated the devel-opment of new solutions (3537).
Traditional antibiofouling surfaces are fundamentally in solidforms (i.e., their surface atoms/molecules are static or quasi-staticin nature). Therefore, permanent interactions between the solidsurfaces and the biological adhesives can eventually be estab-lished depending on the time scales of the adhesion processes,which then lead to stable attachment and biofouling. Creatinga surface that possesses dynamic features down to the nanometerscale, i.e., mobility of surface molecules or structures, may inhibitthese permanent interactions, thereby significantly disrupting thebiological adhesion. A potential approach to generating dynamicsurfaces is to utilize a stabilized liquid interface. Inspired by theNepenthes pitcher plant (38), we recently developed a new modelof omni-repellent surface, one based not on an unstable and tran-sient solid-air Cassie-type interface, but rather on a stable, immo-bilized, and smooth liquid surface locked in place by a speciallydesigned porous solid, allowing the material to function evenwhen submerged (39). This novel slippery liquid-infused poroussurface (SLIPS) is a material concept that exploits the extremestability of the fully wetted liquid film to maintain repellencyacross a broad range of temperature, pressure, surface tension,and other conditions (39). Spec